Professor, Institute of Industrial Science, University of Tokyo, Tokyo 1
KODANSHA LTD., Tokyo
ELSEVIER SCIENCE PUBLISHERS B. V., Amsterdam
exchive sales rights in Jopmr
12-21. Otowa 2-chome, Bunkyo-ku. Tokyoll2, Japan
for the US.A. and Canada
ELSEVIER SCIENCE PUBLISHING COMPANY. INC. 655 Avenue of the Americas, New York, NY 10010, U.S.A.
for the resr ofrhe world
ELSEVIER SCIENCE PUBLISHERS B. V.
25 Sara Burgerhanstraat. P.O. Box 21 1, 1000 AE Amsterdam, The Netherlands
Library of Congress Cataloglng-in-Publication Data
Suzukl. Motoyukl. 1941-
Adsorptton englneerlng / Motoyukl Suzukl.
--(Chemical englneerlng monographs : vol. 25)
Includes bibllographical references ISBN 0-444-98802-5 (U.S.)
1. Adsorptlon. I. Tttle. 11. Series Chemical e n g l n e e r l n g nonographs : v . 25. TP156.A35S89 1989 660'.28423--dc20 89-23532 CIP ISBN 0-444-98802-5 (Vol. 25) ISBN 0-444-41 295-6 (Series) ISBN 4-06-201 485-8 (Japan) Copyright @ 1990 by Kodansha Ltd. All rights reserved.
No part of this book may be reproduced in any form, by photostat, microfilm. retrieval system, or any other means, without the written permission of Kodansha Ltd. (except in the case of brief quotation for criticism or review).
CHEMICAL ENGINEERING MONOGRAPHS
Advisory Editor: Professor S.W. CHURCHILL, Department of Chemical Engineering, University of Pennsylvania, Philadelphia, PA 19104, U.S.A Vol. 1 Polymer Engineering (Williams)
Vol. 2 Filtration Post-Treatment (Wakeman) Vol. 3 Multicomponent Diffusion (Cussler) Vol. 4 Transport in Porous Catalysts (Jackson)
Vol. 5 <alculation of Properties Using Corresponding-State Methods (Sterktek et 01.)
Vol. 6 Industrial Separators for Gas Cleaning (Storch et 01.) Vol. 7 Twin Screw Extrusion (Janssen)
Vol. 8 Fault Detection a n d Diagnosis in Chemical and Petrochemical Processes (Himmelblau)
Vol. 9 Electrochemical Reactor Design (Pickett) Vol. 10 Large Chemical Plants (Froment, editor) Vol. 1 1 Design of lndustrial Catalysis (Trimm)
Vol. 12 Steady-state Flow-sheeting of Chemical Plants (Benedek, editor) Vol. 13 Chemical Reactor Design in Practice (Rose)
Vol. 14 Electrostatic Precipitators (Bohm)
Vol. 15 Toluene, the Xylenes a n d their lndustrial Derivatives (Hancock, editor) Vol. 16 Dense Gas Dispersion (Britter and Griffiths, editors)
Vol. 17 Gas Transport in Porous Media: The Dusty Gas Model (Mason and Malinauskas)
Vol. 18 Principles of Electrochemical Reactor Analysis (Fahidy) Vol. 19 The Kinetics of lndustrial Crystallization (Njrvlt et 01.)
Vol. 20 Heat Pumps in Industry (Moser and Schnitzer)
Vol. 21 Electrochemical Engineering (RouSar et 01.) in 2 volumes: Parts A-C and Parts D-F
Vol. 22 Heavy Gas Dispersion Trials at Thorney Island (McQuaid, editor) Vol. 23 Advanced Design of Ventilation Systems for Contaminant Control
Vol. 24 Ventilation '85 (Goodfellow, editor) Vol. 25 Adsorption Engineering (Suzuki)
1 was introduced to adsorption when 1 spent two years (19691 1971) with Professor J. M. Smith at the Universityof California, Davis, studying application of chromatographic methods to determine rate processes in adsorption columns. After returning to the lnstitute of Industrial Science, University of Tokyo, 1 joined Professor Kunitaro Kawazoe's adsorption research group where pioneering work in adsorption engineering had been conducted, and started research on development of adsorption technology for water pollution control.
Since then I have had many opportunities to acquire valuable ideas on adsorption problems not only from Professor Kawazoe but from numerous other senior colleagues including Professor Toshinaga Kawai of Kanagawa University, Professor Yasushi Takeuchi of Meiji University and the late Professor Hiroshi Takahashi of I.I.S., University of Tokyo.
In the laboratory, I was fortunate to have many good collaborators including Dr. Kazuyuki Chihara, Dr. Dragoslav M. Misic, Professor Byun-Rin Cho, Dr. Akiyoshi Sakoda, Dr. Ki-Sung Ha and other students. The technical assistance of Mr. Toshiro Miyazaki and Mr. Takao Fujii in laboratory work was invaluable. This volume was written based on the work of this group and 1 am very grateful to these colleagues and to many others not listed here.
In preparing the manuscript, I repeatedly felt that much work remains to be done in this field and that many directions of research are waiting for newcomers to seek out. Because of my imperfect knowledge and experience, many important problems which require discussion are not included. If possible these should be treated in a future edition. It took me far longer than expected at the beginning to prepare the manuscript for this monograph mainly due to idleness. Mr. Ippei Ohta of Kodansha Scientific Ltd. diligently prodded me. Without his energy this book would never have been completed. I also had to spend much time working at home and I am very grateful to my patient and gentle wife, Keiko, to whom I dedicate this volume.
. . .
. . .
. . .
. . .
. . .
. . . .
. . .
. . ..1
. . .
. . .
. . .
. . .
. . .
. . . .. 5 2 1 Activated Carbon 8
2 2 Slllca and Alumlna IS 2 3 Zeollte 16
2 4 Other Adsorbents 2 1
2 5 Measurement of Pore-related Properties 22
. . .
. . .
. . . .
. . .
. . .
. . .
. . .. 3 5
3 1 Equ~llbr~urn Relatlons 35 3 2 Adsorptlon Isotherms 37 3 3 Heat of Adsorptlon 5 1
3 4 Adsorptlon Isotherms for Multlcomponent Systems 56 3 5 Adsorptlon Isotherms of Unknown Mlxtures 60
4Diffusion in Porous Particles..
. . .
. . ..63 4 1 Dlffuslon Coefficient 63
4 2 Pore D~ffuslon 64 4 3 Surface Dlffuslon 70 4 4 Mlcropore Dlffus~on 85
5Ktnetics of Adsorptlon in a Vessel
. . .
. . .
. . .
. . . ..95 5 I Fundamental Relatlons 95
5 3 Batch Adsorptlon In a Batch with Finrte Volume 106 5 4 Adsorptlon rn a Vessel wlth Cont~nuous Flow 117 5 5 Flurd-to-Partrcle Mass Transfer In a Vessel 118
6Kinetics of Adsorption in a Column-Chromatographic
. . .
. . .
. . .
. . .
. . .
. . . .
. . ..I25 6 I Fundamental Relations 126
6 2 Analysts of Chromatograph~c Elutlon Curves 127 6 3 Method of Moment 128
6 4 Extens~on of the Method of Moment to More Complex Systems 135 6 5 Comparrson wlth Slmpler Models 144
6 6 Other Methods for Handllng Chromatograph~c Curves 148
7Kinetics of Adsorption in a Column-Breakthrough Curves
..I51 7 1 Llnear Isotherm Systems-Solut~on to the General Model 152 7 2 Llnear Isotherm System-Slmple Models 156
7 3 Nonlinear Isotherm Systems-Constant Pattern Adsorptlon Profile 158
7 4 Numerrcal Solutrons for Nonlinear Systems 170
7 5 Breakthrough of Mult~component Adsorbate Systems 172 7 6 D~sperslon and Mass Transfer Parameters In Packed Beds 179
8Heat Effect In Adsorption Operation
. . .
. . .
. . .
8 1 Effect of Heat Generation on Adsorptlon Rate Measurement by a Srngle Partrcle Method 187
8 2 Basic Models of Heat Transfer In Packed Beds 190 8 3 Heat Transfer Parameters rn Packed Beds 193
8 4 Chromatographic Study of Heat Transfer In Packed Beds of Adsorbents 197
8 5 Adrabat~c Adsorptlon rn a Column 201
8 6 Adsorptlon wrth Heat Transfer Through the Wall 203
9Regeneration of Spent Adsorbent
. . .
. . ..205 9 1 Thermal Desorptlon in Gas Phase 206
9 2 Chemlcal Desorptlon from a Column 208
9 3 Thermal Regeneration of Spent Actrvated Carbon from Water Treatment 214
. . .
. . . .,229 10.1 Basic Relations of Chromatographic Elution Curves in Linear Isotherm
10.2 Separation of the Neighboring Peaks 232 10.3 Large Volume Pulses 233
10.4 Elution with Concentration Gradient Carrier 236 10.5 Chromatography for Large-scale Separation 238
1 1Pressure Swing Adsorption
. . .
. . .
. . . ..245 I I . I General Schema of PSA Operation 246
11.2 Equilibrium Theory for PSA Criteria 250
11.3 Numerical Solution of Nonequilibrium PSA Model 253
11.4 Simplified Solution of Dynamic Steady State Prome from Continuous Countercurrent Flow Model 259
11.5 Mass Transfer Coefficient ln Rapid Cyclic Adsorption and Desorption 267
11.6 PSA Based on Difference of Adsorption Rates 271
12Adsorption for Energy Transport
. . .
. . .
. . .
..275 12.1 Principle of Adsorption Cooling 275
12.2 Choice of Adsorbate-Adsorbent System 277
12.3 Analysis of Heat and Mass Transfer in a Small-scale Adsorption Cooling Unit Utilizing Solar Heat 280
12.4 Heat Pump Utilizing Heat of Adsorption 287 Index 291
Understanding of engineering design methods of adsorption systems is an important aspect of process engineering design not only in the chemical industry but also in the fields of environmental pollution control and energy utilization. Moreover, adsorption is coming to be regarded as a practicable separation method for purification or bulk separation in newly developed material production processes of, for example, high-tech materials and biochemical and biomedical products.
Advances in chemical engineering principles such as transfer rate processes and process dynamics and accumulation of quantitative data in the field of adsorption, together with the development of easily accessible microcomputers, have combined to enable the development of an integrated curriculum of adsorption engineering.
The first book on engineering design of adsorption apparatus in Japan, written by Professor Kunitaro Kawazoe (1957), was published as part of the "Advanced Series in Chemical Engineering." The contents included: I. Adsorbents, 2. Industrial Adsorbers, 3. Adsorption Equilibrium, 4. Adsorption Rate, 5. Contact Filtration Adsorption, 6. Moving Bed Adsorption, 7. Fixed Bed Adsorption, and 8. Fluidized Bed Adsorption. For many adsorption design engineers, this was the only textbook for a long time. Later developments in the field have been published in Kagaku-kogaku-benran (Chemical Engineering Handbook edited by the Society of Chemical Engineers, Japan). This is a good contrast with Perry's Chemical Engineers' Handbook up to 6th editions where the works of the school of the late Professor Theodore Vermeulen were introduced.
A number of volumes have been written on adsorbents and adsorption. The one by professor D. M. Ruthven (1985) is a good compilation of the chemical engineering work conducted in this field. Extensive work on diffusion in zeolite by the author and his collaborators are summarized and a complete collection of mathematical analyses in the literature are useful for readers initiating advanced studies in this field. Also Professor R. T. Yang (1986) published a book focusing on gas separation by
adsorption, which is also a good reference for chemical engineers. The purpose of the present volume is to provide graduate students and chemical process engineers an overall understanding of the chemical engineering principles related to adsorption processes. Balanced rather than detailed discussions are attempted.
Chapter 2 gives brief picture of the adsorbents frequently used in actual processes. Surface characteristics and pore structures of adsorbents are the main properties in determining adsorption equilibrium and rate properties which are needed for plant design. New adsorbents are continuously being developed, introducing new applications for adsorption technology.
Chapter 3 introduces the concepts of adsorption equilibrium with the primary purpose of discussing the applicabilities and limits of some simple expressions which are used in later sections on design of adsorbers. Adsorption equilibrium is the fundamental factor in designing adsorption operations.
Chapter 4 is an attempt to provide an global view of diffusion phenomena in adsorbent particles, another important aspect of adsorp- tion engineering.
Chapter 5 deals mainly with batch adsorption kinetics in a vessel. Determination of intraparticle diffusion parameters should be done with a simple kinetic system where no other rate processes are involved. For this purpose measurement of concentration change in the finite bath where adsorption takes place is the most effective method. Concentration change curves derived for nonlinear isotherm systems as well as for a linear isotherm system are presented for convenient determination of rate parameters. These discussions are also applicable to the analysis and design of adsorption operation in a vessel o r differential reactor.
Chapter 6 introduces another powerful technique for determining the rate parameters involved in an adsorption column. The principle of chromatographic measurement implicitly contains many fundamental concepts concerning dynamic performance of a column reactor. The mathematical treatments introduced in this chapter can easily be extended to cover more complicated dynamic operations.
Chapter 7 gives the basic relations used for calcu!ation of breakthrough curves in an adsorption column. The discusssion focuses on simpler treatment with overall mass transfer parameter. There are many rigorous solutions to fundamental equations but in most industrial designs, while a quick estimation method is preferable at the same time the effects of many parameters need to be clarified. Constant pattern development is an important characteristic in the case of nonlinear (favorable) isotherm systems simplifying design calculation.
Heat effects in adsorption processes are discussed in Chapter 8. Adsorption is accompanied by heat generation, and adsorption equilibrium and rate are dependent on temperature. This coupling effect brings about complex but interesting problems.
Chapter 9 is devoted to methods for the regeneration of spent adsorbents. Since adsorption separation is a transient technique, regeneration of adsorbents after the period of adsorption is an important part of an adsorption purification or separation system. Recovery of valuable adsorbates will also become increasingly important.
In Chapter 10, chromatographic operations on the industrial scale is considered. Development of this area is especially needed in the area of fine products separation such as required in biotechnological processes. Much improvement of adsorbents and new operation schemes are expected in this field.
Chapter 1 I introduces a bulk separation technique, pressure swing adsorption (PSA). This method has become very sophisticated and complex. The chapter attempts to define fundamental ideas in considering these attractive processes.
In Chapter 12, one unique application of adsorption for energy utilization purposes is introduced. For refrigeration, cooling and heat pumping application of adsorption phenomena has been attempted. Fundamental ideas on these application are discussed.
As described above, Chapters 2 through 4 deal with the fundamentals of adsorption phenomena which are necessary to understand the operation and design of basic adsorption operations introduced in Chapters
5to 7. Chapters 8 and 9 are fundamental topics specific to adsorption operations and Chapters 10, 11 and 12 introduce basic ideas on the practical and rather new applications of adsorption phenomena. The reader can start from any chapter of interest and refer to the fundamentals if necessary.
Physical adsorption is caused mainly by van der Waals force and electrostatic force between adsorbate molecules and the atoms which compose the adsorbent surface. Thus adsorbents are characterized first by surface properties such as surface area and polarity.
A large specific surface area is preferable for providing large adsorption capacity, but the creation of a large internal surface area in a limited volume inevitably gives rise to large numbers of small sized pores between adsorption surfaces. The size of micropore determines the accessibility of adsorbate molecules to the adsorption surface so the pore size distribution of micropore is another important property for characterizing adsorptivity of adsorbents.
Also some adsorbents have larger pores in addition to micropores which result from granulation of fine powders o r fine crystals into pellets or originate in the texture of raw materials. These pores called macropores are several micrometers in size. Macropores function as diffusion paths of adsorbate molecules from outside the granule to the micropores in fine powders and crystals. Adsorbents containing macropores and micropores are often said to have "bidispersed" pore structures.
Pore size distributions of typical adsorbents are shown in Fig. 2.1. Surface polarity corresponds to affinity with polar substances such as water. Polar adsorbents are thus called "hydrophilic" and aluminosili- cates such as zeolites, porous alumina, silica gel or silica-alumina are examples of adsorbents of this type.
On the other hand, nonpolar adsorbents are generally "hydrophobic." Carbonaceous adsorbents, polymer adsorbents and silicalite are typical nonpolar adsorbents. These adsorbents have more affinity with oil than water.
Popular adsorbents in commercial use are reviewed in the following sections. Measurement techniques for pore size distributions are also briefly introduced in the later sections of this chapter.
( a ) Actlvatcd carbons
Fig. 2.1.a. Pore size distnbution of typ~cal activated carbons.
Pore rad~us, r, ( A )
( b ) Acttvated carbons
Fig. 2.1.b recover
Activated Carbon 7
10 20 50 100 200 500 10' Pore rad~us r,
Fig 2 I c Pore slze distributions of Sllica gel (A) Type A, (B) Type B
F I ~ 2 1 d Pore size dlstrlbut~ons of Alumma pellets w ~ t h d~lferent pelletizing pressures Pellet density 1 0 58, 2 0 68 3 0 83 4 1 02 g/cm'
Pore rad~us. r,
( A )
h g 2 l e Pore slze dlstnbut~ons of Molecular acve zeol~te 5 A (A)
Davtdson 2-100 (B~nderlcss). (B) Dav~dson Regular.
Act~vated carbons are the microporous carbonaceous adsorbents whose history can be traced back to 1600 B.C. when wood chars were used for medicinal purposes in Egypt. In Japan, a well for underground water equlpped with a charcoal filter at the bottom was found at an old shrine (Kashiwara Jingu, Nara) constructed in the 13th century A. D. In Europe, wood char and later bone char were used for refining beet sugar, a practice started in France because of the blockade against the Continent during the Napoleonic era. In the 20th century, during the World
Wars,the need to develop gas masks stimulated rapid growth In adsorption research. Many books have been published on activated carbon and ~ t s applications (Araki, 1932; Bailleul et at!, 1962; Hassler, 1974; Mantell, 1951; Mattson and Mark, 1971; Tanso Zairyo-Gakkai, 1975.
2.1.1. Preparation of activated carbons
Commercially available activated carbons are prepared from carbon- containing source materials such as coal (anthracite or brown coal), lignite, wood, nut shell, petroleum and sometimes synthetic high polymers
These materials are first pyrolyzed and carbonized at several hundred degrees centigrade During thls process the volatlle fract~on and low molecular products of pyrolys~s are removed and the res~dual carbona-
Activated Corbon 9
ceous material undergo the following activation process by using oxidizing gases, such as steam at above 800°C or carbon dioxide at higher temperatures. Micropores are formed during the activation process. The yield of activated carbon from raw materials is in most cases less than 50% and sometimes below 10%.
Carbonization and activation can also be performed using inorganic chemicals such as zinc chloride or phosphoric acid, which
isknown to have a catalytic effect on pyrolytic condensation of carbohydrates. Then reaction proceeds at lower temperatures and increases yield of char during carbonization. In this process, precursor of micropore is formed when carbonization takes place around fine crystals of inorganic salt and washing of the salt by acid after carbonization produces micropores which are larger in diameter than those formed by gas phase activation. This method provides the larger micropores preferable for the adsorption of larger molecules.
Micropores, where most adsorption takes place, are in the form of two-dimensional spaces between two graphite-like walls, two-dimen- sional crystallite planes composed of carbon atoms. The distance between the two neighboring planes of graphite is 3.76
A(0.376 nm), but in the case of activated carbons which have a rather disordered crystallite structure (turbostratic structure), this figure must be larger since adsorbate molecules are not accessible otherwise (Fig. 2.2).
B. suface oxide groups
Most activated carbons contain some oxygen complexes which arise from either source materials or from chemical adsorption of air (oxidation) during the activation stage or during storage after activation. Surface oxides add a polar nature to activated carbons, e.g. hydrophicity, acidity and negative [-potential.
Oxygen complexes on the surface exist mainly in the form of four different acidic surface oxides: I) strong carboxylic groups, 11) weak carboxylic groups which exist as lactone groups combined with the neighboring carbonyl groups, 111) phenolic groups and 1V) carbonyl groups which form lactone groups with carboxyl groups of Type I1 (Fig. 2.3).
Distinguishing these acidic oxides is possible by multibasic titration (Boehm et a!., 1964), titration with alkaline solutions of different
Fig. 2.2. Graph~te structure (a,b) and turbostratic structure (c). Cenceptual ~llustration of granular activated carbon (d).
strength. For instance, sodium bicarbonate, NaHCO3, whose pK, value is 6.37, neutralizes surface oxides of group (I). Sodium carbonate, NalCO, (pK.=10.25), can be used for titration of groups (I) and (II), sodium hydroxide, NaOH (pk;=15.74), for groups (I), (11) and (111) and sodium methoxide, NaOC2H5 (pR=20.58), for groups (I), (II), (111) and (IV). Hence it is possible to determine the amount of each surface oxide group from the difference in titration values.
There are several other forms of oxides including basic groups such as cyclic ether groups. The basic character of activated carbon is emphasized when activation is conducted at higher temperatures.
Surface oxide groups can be removed by heat treatment of carbons in an inert atmosphere or under vacuum (Puri et of., 1962. 1964, 1966). Evolution of COz is observed at temperatures below 600°C and surface acidity 1s closely related to the amount of the evolved C02.
Actiwted Carbon I I
Open lYPe Lactonc type
Fig. 2.3. Surface oxides on carbon surface. I : Carboxyl group, a : Removed by 200°C, b : Removed above 325OC. 11 : Carboxyl group which exists as lactol group, 111 : Phenolic hydroxyl group, I V : Carbonyl group.
Above 600°C, the evolving C O is considered to correspond to the basic functional groups on the carbon suiface.
Activated carbon also contains to some extent ashes derived from starting materials. The amount of ash ranges from 1% to 12%. ,Ashes consist mainly of silica, alumina, iron, alkaline and alkaline earth metals. The functions of these ashes are not quantitatively clarified but some of them are 1) increasing hydrophilicity of activated carbon, which is advantageous when PAC is used for water treatment, 2) catalytic effects of alkaline, alkaline earth and some other metals such as iron during activation or regeneration step which modifies pore size distribution to larger pore range, and so on. Acid soluble ashes can be removed by washing with weak acid.
2.1.3.Powdered activated carbon ( P A C )
Activated carbons in commercial use are mainly in two forms: powder form and granular or pelletized form. Powdered activated carbons (PAC) in most cases are produced from wood in the form of saw dust. The average size of PAC is in the range of 15 to 25 pm and the geometrical standard deviation is between 0.15 to 0.266. This particle size assures that intraparticle diffusion will not be the rate limiting step; thus the adsorption operation is designed from the view point of selection of
contacting apparatus, mixing of PAC with liquid, separation of PAC after contacting and disposal or regeneration if possible after usage.
The major industrial uses of PAC are decolorization in food processes, such as sugar refinery, oil production and sodium glutamate production as well as wine preparation. Recently, considerable PAC is used in water treatment for both drinking water and wastewater treatment.
In the use of PAC in water phase, surface charge of the carbon powder becomes an important factor since it affects ease of coagulation sedimentation or filtration for separation of PAC from the bulk liquid after adsorption. Surface charge can be detected by [-potential or colloid titrations. Measurement of [-potential for several commercially available PACs showed that it varies considerably by sample and that it is also very dependent on pH of the solution, suggesting that the existence of dissociative functional groups (oxide groups) is playing an important role. The effects of the acid washing for removing soluble ashes and the successive heat treatment to remove surface acidic oxides
Fig 2 4 Change of [-potentla1 of PAC by a c ~ d treatment (HCI I N) and heat treatment (900°C, N > stream) P A C Hokuetsu Tanso, wood char
(Reproduced w ~ t h permission by S u z u k ~ , M and Ch~hara, K , Wafer Res, 22. 630 (1988))
Acfivaed Carbon 13
on [-potential are clearly shown in Fig. 2.4. Powdered activated carbons produced from saw dust are used and 5-potential calculated from the electromobility of the powders at different levels of pH are illustrated in the figure. Presence of both acid soluble ashes and surface oxides increases the negative charge of the particles; this is not desirable when coagulation of the powders is needed.
When PAC is used, not only is its adsorbability utilized but its surface charge may also cooperate as a coagulant for colloidal fractions in the liquid phase. In this case, however, the regeneration of PAC may become rather difficult. This is one of the reasons why spent PAC is in most cases dumped rather than regenerated for repeated use.
2.1.4.Granular activated carbon
Granular activated carbons (GAC) are either in the form of crushed granules (coal or shell) o r in the pelletized form prepared by granulation of pulverized powders using binders such as coal tar pitch. GAC produced from petroleum pitch is prepared by activation of the spherical beads prepared from the pitch.
Size of granules differ depending on the application. For gas phase adsorption, cylindrically extruded pellets of between 4 to 6mm or crushed and sieved granules of 4/ 8 mesh to
lo/20 mesh are often used. The main applications in gas phase are solvent recovery, air purification, gas purification, flue gas desulfurization and bulk gas separation.
In the case of liquid phase adsorption, intraparticle diffusion often becomes the rate determining step of adsorption so smaller particles of for example, 12/42 mesh are advantageous from this point of view, but operational requirements such as ease of handling, low pressure drop in the adsorption bed, little elutriation or abrasion during back washing and so on define the lower limit of the particle size. Decolorization in sugar refinery, removal of organic substances, odor and trace pollutants in drinking water treatment, and advanced wastewater treatment are major applications of liquid phase adsorption.
Spent GAC in most applications is regenerated by a thermal method. Detailed discussions are given in Chapter 9.
2 . 1 .Carbon molecular sieves
Size of micropore of the activated carbon is determined during pyrolyzing and activation steps. Thus small and defined micropores that have molecular sieving effects can be prepared by using proper starting materials and selecting conditions such as carbonizing temperature,
activation temperature and time or properties of binders for granulation. The main applications of activated carbon with molecular sieving ability are separation of nitrogen and oxygen in air on the basis of difference of diffusion rates of these gases in small micropores, and adjustment of fragrance of winery products where only small molecules are removed by adsorption in liquid phase.
Carbon molecular sieve (CMS, or Molecular Sieving Carbon, MSC) is an interesting material as a model of activated carbons since it has a uniform and narrow micropore size distribution. The Dubinin-Astakhov Equation for adsorption isotherms of various gases was tested using MSC (Kawazoe et a/., 1974), and later this equation was extended for adsorbents with micropore size distributions (Sakoda and Suzuki, 1983) and for isotherm relation in the low pressure range. Also, chromatographic measurement of Henry's constants and micropore diffusivities were made for MSC (Chihara et al., 1978); these gave clear relations between heat of adsorption and activation energy of diffusion in micropores of MSC.
2.1.6.Activated carbon fiber
Synthetic fibers such as phenolic resin (Kynol R), polyacrylic resin (PAN) and viscose rayon are carbonized at high temperatures in inert atmosphere and activated carbon fiber (ACF) is then prepared by careful activation. Recently the carbon fibers prepared by spinning from mesophase carbon melt derived from coal tar pitch are being further activated to provide ACF at less cost.
Most ACFs have fiber diameter of 7 to 15 pm
,which is even smaller than powdered activated carbon. Hence the intrafiber diffusion becomes very fast and the overall adsorption rate is controlled in the case of ACF bed, by longitudinal diffusion rate in the bed (Suzuki and Sohn,1987).
ACF is supplied in the form of fiber mat, cloth and cut fibrous chip of various sizes. ACF and cellulose composite sheet is also available.
Application of sheet adsorbent is found in the field of air treatment such as solvent recovery. Application in water treatment is under development in several areas such as chlorinated organics and odorous components removal during city water purification from deteriorated water sources such as eutrophicated lake water and polluted under- ground water (Sakoda et a!., 1988).
S111ca and Alwnina I 5
Silica and Alumina
Pure silica, Si02, is naturally a chemically inactive non-polar material like quartz but when it has a hydroxyl functional group (silanol group), the surface becomes very polar and hydrophilic (Fig. 2.5).
Silica gel is the adsorbent particle prepared by coagulation of a colloidal solution of silicic acid (3 to 5 nm) followed by controlled
Fig. 2.5. Surface hydroxyl group on sll~ca surface.
Fig 2 6 Typ~cal examples of a d s o r p t ~ o n t~othcrms of water vapor on Silica
dehydration. Liquid sodium silicates are neutralized by sulfuric acid and the mixture is then coagulated to form hydrogel. The gel is washed to remove the sodium sulfate formed during the neutralization reaction. Then it is dried, crushed and sieved. Spherical silica gel particles are prepared by spray drying of the hydrogel in hot air.
Silica gels of two types of pore size distribution are frequently used for commercial purposes. Type A and B have different shapes of adsorption isotherms of water vapor (Fig. 2.6). This difference originates from the fact that type A is controlled to form pores of 2.013.0 nm while Type B has larger pores of about 7.0 nm. Internal surface areas are about 650 m2/g (Type A) and 450 m2/g (Type
Silica gel contains about 0.04 to 0.06 gso/g of combined water after heating at 350°C and if it loses this water, it is no longer hydrophilic and loses adsorption capacity of water.
The main application is dehumidification of gases such as air and hydrocarbons. Type A is suitable for ordinary drying but Type B is more suitable for use at relative humidity higher than 50%.
Aluminum oxides have several crystal forms. Active alumina (porous alumina) used as an adsorbent is mainly y-alumina. Specific surface area is in the range of I50 and 500 m2/g with pore radius of I5 to 60
A(1.5 to 6 nm), depending on how they are prepared. Porosity ranges from 0.4 to 0.76 which gives particle density of 1.8 to 0.8 g/cm3.
Porous alumina particles are produced by dehydration of alumina hydrates, in most cases alumina trihydrate, Alz033H20, at controlled temperature conditions to about 6% of moisture content.
Active alumina is also used as a drying agent and the typical adsorption isotherm of water vapor is included in Fig. 2.6. It is also em- ployed for removal of polar gases from hydrocarbon streams.
Zeolite (the word derives from a Greek word zeein meaning to boil) is an aluminosilicate mineral which swells and evolves steam under the blowpipe. More than 30 kinds of zeolite crystals have been found in natural mines. Many types can be synthesized industrially.
Crystalline structures are composed of tetrahedral units, at the center of which a silicon (Si) atom is located with four oxygen atoms surrounding it. Several units construct secondary units, which are
Frg 2 7 Several fundamental unlts of SI atoms In Zeolrte structures Nerghborrng S I atoms are connected through oxygen atom not shown In the figure
llsted In Fig 2 7 Arrangement of these secondary unrts forms regular crystalllne structures of zeol~tes
Regular crystalllne structures prov~de unlque adsorpt~on character- ~stlcs For example, m the case of zeol~te type A, e~ght sodal~te units, (a) In Fig 2 8, form a cublc cell whose unlt s ~ d e 1s 12 32
sodal~te unlt 1s located at the corner Neighboring un~ts are connected through the D4R unlt (Fig 2 7 d) rn the form of (c) In Fig 2 8 and the resulting erght-membered rlng connecting ne~ghbonng cells controls accesslbll~ty of adsorbate molecules Into the cell where adsorpt~on takes place In the case of zeol~te type X or Y sodal~te unlts are connected through D6R (Flg 2 7 e) unlts and form the unlt structure shown by F I ~ 2 8 e A cell In the unlt shown by F I ~ 2 8 f has four openlngs composed of I 2-membered nngs
SI atoms In tetrahedral unlts can be replaced by alumlnum (Al) Ion whlch results
ma deficit of positive valence, requlrlng the addit~on of catlons such as alkallne or alkallne earth Ions corresponding to the number of Al atoms These catlons are easlly exchangeable and the slze and properties of these Ions mod~fy adsorption character~stlcs of zeol~tes slnce they affect the sue of the wlndow between the cells
2 3 1
Zeollte mlned I n Japan and nelghborlng countries 1s llm~ted In type and only cl~nopt~lollte and rnorden~te are now excavated (Mlnato 1967)
(a) Sodal~te unrt (&cage) (SI, A1 atoms (b) Sodallte unlt ( w ~ t h oxygen atoms) are shown)
(c) Type A structure unlt Composed (d) M~cropore cell I n Type A unlt-a of erght sodalrte unlts (only SI, A1 cage, gas molecules enter through atoms are shown, black circles are on e~ght-membered nngs
(e) Type X and Y structure unit, composed of 10 sodal~te units connected by W R units
(I) M~cropore cell in Type X(Y) unlt, gas molecules enter through twelve-membered rlngs
F I ~ 2 R Ftructurc unlt o f sodalite ((a) and (b)). Type A ((c) and (d)). X(Y)
The main uses of natural zeolite as adsorbent are as drying agents, deodorants, adsorbents for air separation, ion exchangers for water purification especially for removing ammonium ion and heavy metal ions and for water softening, soil upgrading and so on.
Suzuki and Ha (1985) showed that clinoptilolite has good adsorp- tion selectivity of ammonium ion and obtained the adsorption equilibrium and rate of ammonium exchange.
Some zeolitic crystal structures can be synthesized by hydrothermal
R g 2 9 Relat~ons between effectlve pore size o f Zeol~tes A and X and Lennard-Jones klnet~c d~ameter, o Reproduced w ~ t h permlsslon from Breck, D W
.Zeolrre Molecular Sieve-srmcture, Chernrsrry and Use, J Wlley and Sons, N e w York (1974)
(Reproduced w ~ t h permlss~on by Ruthven, M
.Prmcples of Adrorprron & Adr Processes. I I , Wlley (1985))
reaction in autoclaves. Much of the literature is devoted to clarifying crystal structure and synthesis (Barrer 1968, Flanigan and Sand 1971, Breck 1973, Meier and Uytterhoeven 1973, Katzer 1977, Barrer 1982, Olson and Bisio 1984, Ramoa el al. 1984, Drzaj el al. 1985, Murakami el al. 1986).
A limited nurnber of synthetic zeolites are currently used as commercial adsorbents i.e., Type A and Type X.
In the crystal structures of Type A, shown in Fig. 2.8, exchangeable cations are located near the window between neighboring cells. The 4A type zeolite contains Na ion at this site, which permits the entry of molecules smaller than 4
A.This effect is called the molecular sieving effect, and is schematically illustrated in Fig. 2.9. If the K ion, which is larger than the Na ion, is introduced to this position, effective window (aperture) size becomes 3
Hz0and NH3 can penetrate through the window. Then this type is called 3A zeolite. On the other hand, if a Ca ion, which has two valences, is introduced, the effective aperture becomes larger. The zeolite of this type is called 5A zeolite.
Type X zeolite has much larger windows made up of 12-membered rings (Fig. 2.8). and is usually called 13X zeolite.
In sugar refineries, bone char has been commonly used as an adsorbent for decolorizing and refining sugar since the 19th century. Bone char is believed to have basically the same adsorption character- istics as activated carbons. But in addition to the ion exchange abilities derived from the main constituent, calcium hydroxy apatite functional groups from animal matter may render superior adsorption ability for removing color, odor and taste.
Dry bones free of flesh together with fat and oil of animals crushed, screened and freed from miscellaneous foreign elements are put in an airtight iron retort and heated at 600-900°C for about 8 h. The volatile gases evolved by this process contain ammonium, tar and non- condensible gas. The remaining char is cooled in inert atmosphere then taken out for further crushing and screening. The yield of bone char is about 60%.
Calcium hydroxyapatite is an interesting adsorbent which collects cations of heavy metals such as lead and cadmium. Suzuki (1985) suggested that hydroxyapatite is capable of ion exchange not only with
cations but also with anions such as fluoride ion. The same effects may be expected in part of the hydroxyapatite composing bone chars.
Metal oxides appear to be simple inorganic materials having well- defined chemical structures. However, as far as adsorption on oxide surface is concerned, surface properties, which is largely dependent on how the oxide is prepared, reveal very complicated functions. This is well known in the preparation of metal oxide catalysts.
Metal oxides developed for industrial adsorbents include magnesium oxide, titanium oxide, zirconium oxide and cerium oxide. Magnesium oxide (magnesia) is used for removing polar molecules such as color, acids, and sulfide compounds from gasoline and solvent for drycleaning purposes. Also it is effective in removing silica from water, and magnesium trisilicate is used as a medicinal adsorbent. Ikari (1978) showed that magnesium hydroxide is a good adsorbent for phosphate removal in the advanced treatment of wastewaters.
Oxides of four valence metals, titanium, zirconium and cerium, sometimes show selective adsorption characteristics in removing anions from water phases. Hydrous titanium oxide is known to be a selective adsorbent for recovering uranium in seawater, which is present in the form of carbonyl complex in concentrations as low as 3.2 ppb.
Zirconium oxide in a monohydrated form is found to adsorb phosphate ion from wastewaters (Suzuki and Fujii, 1987). Cerium oxide is effective in adsorption of fluoride ion in industrial wastewaters.
2.5. Measurement of Pore-related Properties
Porosity of adsorbents is determined by several alternative methods. When true solid density, p, (glcm]), is known, total porosity, E I (-), or
specific pore volume, v, (cm3/g), is calculated from p, and particle density, pp (g/cm3), as
Particle density, p,, can be determined using a mercury pycnometer by assuming that mercury does not enter any pore of the porous sample.
Measurement of Pore-related Propertres 23 When the sample is first evacuated and the evacuated sample is exposed to mercury at atmospheric pressure, P., then mercury can penetrate pores with radius larger than 7.5 pm. Most porous adsorbents have intraparticle pores smaller than this and one atmosphere is enough to fill the void between particles with mercury. Thus, by comparing the weight of the empty glass pycnometer filled with mercury, W,, and that of the pycnometer with the sample of weight, W,, filled with mercury after evacuation, W,, the particle density, p,, is calculated as
p, = particle weight] particle volume
where p~~ is the density of mercury at the measurement temperature. True solid densities, p,, are often found in the literature. But some porous bodies are not easy to find in the tables or to make an estimation because they have confined pores which are not accessible from outside. In such cases, the "true" density must be determined by direct measurement.
One practical method is to use the same method as described for measuring particle density using mercury, except that mercury is replaced by a liquid which penetrates pores. Water and organic solvents are often used. The same equation can be used by replacing p, with the density of the liquid employed.
Another method is to employ a helium densitometer (Fig. 2.10). This method is based on the principle of PV=constant at constant temperature. A known weight, W,, of porous sample is put into then evacuated from a closed vessel of volume VI. Next nonadsorbable gases such as helium are introduced to pressure P1, the valve closed and the volume of the vessel changed by moving the piston in the connected cylinder. From the displacement of the piston, the change in volume, AV, and change in pressure, AP, are obtained. Then the volume of the sample, V,, in which helium cannot penetrate is obtained as
and true density, p,, is defined as
Obviously, adsorbable or condensable gases cannot be employed in this method.
Pore size distribution
The most common methods to determine pore size distributions are the A. mercury penetration method,
B.nitrogen adsorption method, and C. molecular probe method.
A. mercury penetration method
By applying pressure,
P,to mercury surrounding a porous body, mercury penetrates into the pores whose radii are larger than r given by
the following equation
r = - 20 cos
where a represents the surface tension of mercury, 470dynelcrn (298 K), 8 is the contact angle between mercury and the sample
Electr~c br~dge Pressure
Constant temperature bath
Measurement of Pore-related Properties 25 surface, which is usually taken as 140°C. Then
An example of a mercury porosimeter is illustrated in Fig. 2.11. A small amount of a sample is put in t o the penetometer, then evacuated, after which mercury is introduced from the separate vessel. Then the penetometer is set in the pressure vessel shown in the figure and high pressure is applied by oil pressure pump. Mercury penetration is detected from displacement of meniscus a t the burette of the penetometer. The pore size distribution is calculated from the pressure- penetration volume relation.
An ordinary mercury porosimeter generates pressure as high as 3000 kg/cm2, which makes it possible to determine pore size distribu- tions down to r-25
A.Usually, this method is suitable for determining larger pores such as macropores of activated carbons.
B. nitrogen adsorption merhod
When nitrogen adsorption is carried out at liquid nitrogen tempera- ture (-195.8OC=77.34 K), nitrogen adsorption on the surface and capillary condensation of nitrogen in the pores take place (Fig. 2.12). The thickness of adsorbed layer on the surface, t, and the size of the pore where condensation happens, rt, depend on the partial pressure of nitrogen. Thus adsorption isotherm can be converted to the pore size distribution by assuming proper relations between both t and r, and the partial pressure, p.
There are several equations proposed for the relation between r and
( d ! ( b )
the pressure, but Halsey's relation is given here as one of the most fundamental relations.
where p, is the saturation pressure, which is the atmospheric pressure in this case.
For the capillary condensation radius, rt, Kelvin radius is derived as
(A)= -9.53 /In@ Ips)
by assuming the contact angle of nitrogen 0 is given as cos 8=1 and the surface tension u=8.85 dynelcm.
Adsorption isotherm of nitrogen at liquid nitrogen temperature is determined by the gravimetric method (Fig. 2.13), o r the constant volume method (Fig. 2.14). From the adsorption isotherm of nitrogen shown in Fig. 2.15, the pore size distribution is calculated by Dollimore method (1964) and shown in Fig. 2.16. Cumulative pore size distribu- tion is sometimes preferred when change of pore size distribution is in- volved, for example during thermal regeneration o r activation of ac- tivated carbons.
For microporous adsorbents such as carbon molecular sieves, Dollimore's method is not advisable since the Kelvin equation is no
Fig 2 13 Gravlmetrlc measurement of nrtrogen adsorpt~on Isotherms a t l l q u ~ d nltrogcn temperature
-Dctccter Nzcyl~nder vw and evacuation i Vacuum Liqu~d nitrogen tank Pump
Frg 2 14 Automatrc adsorptron system for nltrogen (constant volume type), Carlo Erba
Ftg 2 15 Adsorptron ~solherm of nltrogen at Ilquld nltrogen temperature (- 195 8'C)
longer val~d when pore sue 1s close to molecular sue of adsorbate (Dolllmore and Heal, 1964)
For the purpose of descr~b~ng pore size d~stribution In thls range, Horvath and Kawazoe (1983) proposed a method based on potenttal func-
Pore radius, r
Fig 2.16 a Cumulative pore volume (below 100 A) FS 400.
Pore radtus, r ( A )
tion in the pore.
For obtaining an average potential in the slit-like pore between the two layers of carbon, adsorption potential, an expression of adsorbate- adsorbent and adsorbate-adsorbate interactions resulted in the following equation.
where I represents the distance between the nuclei of the two layers, NA and N., respectively, are the number of molecules per unit area of adsorbate and the number of atoms composing the surface layer per unit area, A, and AA are the constants in the Lennard-Jones potential function defined as
where m is the mass of electron, c is the velocity of light, a and
represent the polarizability and the magnetic susceptibility of adsorbent atom (suffix, a) and an adsorbate molecule (suffix, A) and
Kis the Avogadro number. d is defined as
where d, is the diameter of an adsorbent atom and dA is that of an adsorbate molecule.
a is the distance between an adsorbate molecule and adsorbent atom where interaction energy becomes zero and Everett and Pow1 (1976) gave the equation as follows.
By taking proper values for the nitrogen-carbon system as shown in TABLE 2.1, the final form becomes
TABLE 2 1 Phys~cal Propert~es for Pore Size D~stnbutlon Calculat~on by Horvath-Kawazoe Method(1983)
(Reproduced w ~ t h permlsslon by Horvath, G and Kawazoe K , J Chem Eng Japan 16,472 (1983))
TABLE 2 2 Values of Corresponding @/pa). (1-d.) P a ~ r s Accord~ng to Horvath and Kawazoe and Dolllmore
Relat~ve Effect~ve pore sue
P / P ~ - 1 Horvath-Kawazoe model (l-d.) Dolllmorc model
-6 47x10 1 0 43
-2 39x10 6 0 46 - 1 05x10
-1 54x10-4 0 6
-8 86x10 0 7 - 2 95x10 3 0 8
-2 22x10 2 I I 1 16 461x10 1 1 3 1 32 7 59XIC 2 I S 1 46 3 15x10 I 3 0 2 23 7 24x10 1 10 0 5 0 9
(Reproduced w ~ t h permlsslon by Horvath G and Kawazoe, K J Chcm Eng Japan. 16,473 (1983))
where 1 u ln I(
From the equat~on, the relatlon between p and I is unlquely defined and thus the relatlon between the effect~ve pore slze (I-d.) and p is also obtalned as shown In TABLE 2 2 The relatlon IS also plotted in Fig. 2 17
In the table and figure, the pore s u e calculated by Doll~more's method 1s included Both methods approach pore size of around 13 4 I( and
p/p,=O 05, and Howath and Kawazoe suggested that their method should be appl~ed to measurements below p/p,=O 5 and that Dolllmore's method should be used above thls relatlve pressure
Pore size dlstrlbutlons of carbon molecular sleve determlned by thls method are shown In Flg 2 18, where W- 1s the maxlmum pore volume determlned from the amount adsorbed at p/p,=O 9
Measurement o j Pore-related Properties 3 1
Fig. 2.17. Pore size vs. pressure.
(Reproduced with permission by Horvath, G. and Kawazoc. K., J. Ckm fig
Jqpms 16,473 (1983)). 10
-U .: 1.0- ?! P 0. I
Effective pore size (nm)
- x Dollimore
Fig. 2.18. Effective pore size distributions of carbon molecular sieves calculated by Horvath-Kawazoe method.
(Reproduced with permission by Horvath, G. and Kawazoe, K., J. Chem. fig.
Japun. 16,474 (1983)).
10-7 10-6 10-5 1W4 lo-' 10-2 10-1 1.0 Relalive pressure P/P. ( - )
C. molecular probe method
As is understood from Fig. 2.9, for small pores which have molecular sieving abilities, it is not possible to determine pore size distribution by nitrogen adsorption method. In these cases, the most direct determina- tion of the effective pore size is the molecular probe method.
For zeolites, size of entering molecules is determined by assuming that the pores are cylindrical. In the case of activated carbons, especially in the case of CMS, thickness of the molecules decides the adsorbability of the molecules to the micropore since the micropores are considered to be two-dimensional.
Micropore size ( A )
Fig. 2.19. Micropore size distributions of carbon molecular sieve adsorbents determined by the molecular probe method.
sizes is tried (Fig. 2.19). Adsorption from saturated pressures of five organic solvents, carbon disulfide (thickness of 3.7 A), methylene dichloride (4.0 A), ethyl iodide (4.3 A), chloroform (4.6 A) and cyclo- hexane (5.1 A), were tried and from the amount adsorbed of each component, the pore volume for the micropores larger than this size can be determined.
2.5.3. Surface area
lnternal surface area of microporous adsorbents is often used as one of the measures to describe the degree of development of pores. The concept of B.E.T. adsorption isotherm (Eq. 3-12), where the amount adsorbed by monomolecular coverage, q,, is defined, gives the specific surface area by assuming the molecular sectional area of nitrogen to be 16.2 A2/mo1ecu1e, which corresponds to 9.76X104 m2/ mol or 4.35 m2/ Ncc.
T o determine q,,, from the experimentally obtained data of isotherm, so-called BET plot of pr/[q(l-p,)] versus pr is made as shown in Fig. 3.7. Then from the slope and the intersect of the straight line obtained in the range of 0.35<pr<0.5, q, is readily obtained.
In the case of adsorbents with very fine micropores, such as those with molecular sieving effect, it is not easy to make a rigorous definition of the surface area. If BET plot is applied mechanically, "surface area" can
be calculated but the physical meanlng and importance may be reduced. For microporous adsorbents, micropore volumes and size distributions determined by the molecular probe method or the nitrogen adsorption method, if possible, may be more informative than the surface area.
Arakl, T , Karrer~anso (Actrvc Carbon), Maruzen. Tokyo (1932) ( ~ n Japancsc)
Badlcul, G , K Bratzlcr, W Hcrbert and W Vollmer, Aklrw Kohle und Ihrc Induc~nelle Venvendung, 4th Ed , Fcrd~nand Enke, Stuttgart (1962)
Barrcr, R M , Hydro~hemral Chemrrtry of ZPoIr~es, Acadcmrc Press, Ncw York (1982) Barrcr, R M (ed ). Molenrlor Swws, Roc of lhe 1st In1 Zeolrle Confirence, Soc Chem Ind
Boehm, H P , Advances m Calalysu, 16, 179 (1964)
Boehm, H P , E Drchl, W Hcck and R Sappok, Angew Chem , lnt E d , 3,669 (1964) Breck, D W , Zeohte MoImrlor Stew-Stmure, Chemutry and Use. John W~lcy and
Sons. Ncw York (1974)
.M Suzukl and K Kawazoe, AIChE Journal, 24,279 (1982) Dollrmore, D and G R Hcal, J Appl Chem
D a a j , B
.S Hoccvar and S Pcjovnlk (cds). Zeolrtes-Synlhesrr Slnrrrure. Technology and Applrcatton. Elscvlcr, Amsterdam (1985)
Everett, D H and J C Powl, J Chem Soc, Faradoy Tram, 1 72, 619 (1976)
Flanrgan. E M and L B Sand (eds ), M o k ~ h r Srew ZPolrtes-I 8 11, Proc of the 2nd Int Zeolrtc Confcrcncc, Adv m Chemrrtry Serws 101 & 102. ACS (1971)
Hasslcr, J W , hrtfiatron wtlh Actrvared Carbon, Chcm P u b , New York (1974) Howath, Gcza and K Kawazoe, J Chem Eng Japan, 16,470 (1983)
Hara. N and H Takahash1 (cds). Zeorarlo (2iwhtes), Kodansha, Tokyo (1975) (rn Japanese)
.Kagaku to Kogyo, 3 1 , 4 (1978) (In Japanese)
Katzcr, J R (cd ), Molecular Swws 11, Proc of thc 4th Int Zeolrtc Confcmncc, ACS Symposrum Scnes, 40, ACS (1977)
Kawazoc, K , T Kawa~ , Y Eguchl and K Itoga. J Chem Eng Japan. 7, 158 (1974) Mantcll, C L
.Adrorptron, 2nd Ed
.McGraw-H111, New York (1951)
Mattson. J S and Mark, J r , H B
.Actrwted Carbon, Marcel Dekka, Ncw York (1971) Mcrer, W M and J B Uyttcrhoevcn(cds ). Molecular Swws, Proc of the 3rd Int
Zcol~tc Confcrcnce, Adv In ChcmrstrySerlcs 121, ACS (1973)
Mlnato. H , Zeorarto to sono Rryou (Zeolne and rts Applrcatronr), Chapter 2, G~hodo, Tokyo (1967) (m Japancsc)
.A 11j1ma and J W Ward (eds ), New lkwlopmmts m Zoolrte Scwnce and Technology, Proc of the 7th Int Zeollte Conference. Kodansha-Elsev~er, Tokyo/Amstcrdam (1986)
Olson, D and A Bwo (eds ), Rceeedrngs of the Surlh IntornatromI ZEOLITE Conference, Butternorth, London (1984)
Purl, B R (ed ). Roceedrngs of the 5th Confirence on Carbon, vol 1. 165 (1962) Pun, B R and R C Bansal, Carbon, 1,451,457 (1964)
Pun, B R
.Carbon. 4, 391 (1966)
Ramoa, F A E Rodr~gues. L D Rollmann and C Naccache(eds ). Zeobtes Scrence and Technology, NATO AS1 Serlcs E-80 N~jhoff Pub1 The Hague (1984)
Sakoda. A and M Suzuk~, J Chem Eng Japan. 15.279 (1982) Sakoda, A , K Kawazoc and M Suzukr Wafer Re~earch 21, 717 (1987)
Sm~sek, M and S Cerny Acrrbe Corbon Manufaclure Roperttes and Applrcaltons
Suzukl, M and K -S Ha, J. Chem Eng. Japan. 17, 139 (1984). Suzuh, M and J.-E Sohn, 159th ACS Annual Meeting, Denver(1987). Suzukl, M . and T FUJI], Roc 4th APCChE '87, 675, S~ngapore (1987).
Suzukl, M and K Chlhara, Wafer Research. 22,627 (1988).
Suzuk~, T , K. lshlgak~ and N. Ayuzawa, Chem. fig. Commw., 34.143 (1985).
Tanso-za~ryo-gakka~. Karserfan. Kcro f o Ouyou (Acttvated Carbon. FundarnenfaLr and Applrcanons), Kodansha, Tokyo (1975) ( ~ n Japanese)
Zeora~to t o sono R ~ y o u Henshuu Ilnka~, Zeoraifo f o sono Riyou (Zeolite and rfs
In practical operations, maximum capacity of adsorbent cannot be fully utilized because of mass transfer effects involved in actual fluid-solid contacting processes. In order to estimate practical or dynamic adsorption capacity, however, it is essential, first of all, to have information on adsorption equilibrium. Then kineticanalyses are conducted based on rate processes depending on types of contacting processes. The most typical of the rate steps in solid adsorbents is the intraparticle diffusion which is treated in the next chapter.
Since adsorption equilibrium is the most fundamental property, a number of studies have been conducted to determine I) the amount of species adsorbed under a given set of conditions (concentration and temperature) or 2) how selective adsorption takes place when two or more adsorbable components coexist. There are many empirical and theoretical approaches. Only several simple relations, however, can be applied in later treatments on kinetic description of adsorption. These relations are sometimes insufficient for predicting adsorption isotherms under a new set of operating conditions. Thus more sophisticated trials on sound thermodynamics o r on substantial models have been proposed by many authors.
A basic review is given here. For more detailed discussions refer to Ross and Olivier (1964) and Ruthven (1984). A recent publication by Myers (1988) also gives adsorption equilibrium data available in the literature.
When an adsorbent is in contact with the surrounding fluid of a certain composition, adsorption takes place and after a sufficiently long time, the adsorbent and the surrounding fluid reach equilibrium. In this state the amount of the component adsorbed on the surface malnly of the micropore of the adsorbent is determined as shown in Fig. 3.1. The relation between amount adsorbed, q, and concentration In the fluid phase. C. at
Conccntratlon, C or Pressure, p
Fig 3 1 Adsorpt~on ~sotherrns
Ternperaturn, T F I ~ 3 2 Adsorption Isosteres.
temperature, T, is called the adsorption isotherm at T.
The relation between concentration and temperature yielding a given amount adsorbed, q, is called the adsorption isostere (Fig. 3 2).
Adsorprion lsorherms 37 Adsorption isotherms are described in many mathematical forms, some of which are based on a simplified physical picture of adsorption and desorption, while others are purely empirical and intended to correlate the experimental data in simple equations with two o r at most threeempirical parameters: the more the number of empirical parameters, the better the fit between experimental data and the empirical equation. But empirical equations unrelated to physical factors d o not have practical significance since they d o not allow extrapolation beyond the range of variables for which the parameters have been determined.
The simplest model of adsorption on a surface is that in which localized adsorption takes place on an energetically uniform surface without any interaction between adsorbed molecules. When surface coverage or fractional filling of the micropore is 0 (=q/qo) and the partial pressure in the gas phase, p , which is to be replaced by C(= p / R T ) when the concentration in the fluid phase is used, the adsorption rate is expressed as k.p(l
-0) assuming first order kinetics with desorption rate given as kd0. Then equilibration of adsorption rate and desorption rate gives the equilibrium relation as
The above relation is given by Langmuir (1918) and K = k./kd is called the adsorption equilibrium constant.
The above equation is called the Langmuir isotherm. When theamount adsorbed, q, is far smaller compared with the adsorption capacity of the adsorbent, go, Eq. (3-3) is reduced to the Henry type equation;
Further, when the concentration is high enough, p > I
/K, then adsorption sites are saturated and
The above equation is modified when interaction between adsorbing molecules are taken into account. Fowler and Guggenheim (1939) gave
p = -(- I
') exp (2uOlkT) K 1 - 8
where 2u represents pair interaction energy (positive for repulsion and negative for attraction), and k is the Boltsmann constant.
When adsorbed molecules are free to move on the adsorbent surface (mobile adsorption), the Langmuir equation is modified to
When mobile adsorption with interaction is considered, the following is derived.
Fig. 3.3 shows deviation of the isotherm relation from the Langmuir
Flg 3 3 Effcct of moblle adsorpt~on and interaction o f adsorbed molecules o n shape o f Isotherm